Problems arose during research in the 1950s and 1960s. For a while, engineers were faced with what they called "chatter marks" and "devil's scratch" in the inner epitrochoid surface, resulting in chipping of the chrome coating of the trochoidal surfaces. They discovered that the cause was the apex seals reaching a resonating vibration, and the problem was solved by reducing the thickness and weight of the apex seals as well as using more suitable materials. Scratches disappeared after introducing more compatible materials for seals and housing coatings. Yamamoto experimentally lightened apex seals with holes. Now, weight was identified as the main cause. Mazda then used aluminum-impregnated carbon apex seals in their early production engines. NSU used carbon antimony-impregnated apex seals against chrome. NSU developed ELNISIL coating to production maturity and returned to a metal sealing strip for the RO80. Mazda continued to use chrome, but provided the aluminum housing with a steel jacket, which was then coated with a thin dimensional galvanized chrome layer. This allowed Mazda to return to the 3mm and later even 2mm thick metal apex seals.Yamamoto, Kenichi (1971). Rotary Engine. Toyo Kogyo. Page 60-61 Another early problem was the build-up of cracks in the stator surface near the plug hole, which was eliminated by installing the spark plugs in a separate metal insert/ copper sleeve in the housing instead of a plug being screwed directly into the block housing.
Problems arose during research in the 1950s and 1960s. For a while, engineers were faced with what they called "chatter marks" and "devil's scratch" in the inner epitrochoid surface, resulting in chipping of the chrome coating of the trochoidal surfaces. They discovered that the cause was the apex seals reaching a resonating vibration and the problem was solved by reducing the thickness and weight of the apex seals as well as using more suitable materials. Scratches disappeared after introducing more compatible materials for seals and housing coatings. Yamamoto experimentally lightened apex seals with holes. Now, weight was identified as the main cause. Mazda then used aluminum-impregnated carbon apex seals in their early production engines. NSU used carbon antimony-impregnated apex seals against chrome. NSU developed ELNISIL coating to production maturity and returned to a metal sealing strip for the RO80. Mazda continued to use chrome, but provided the aluminum housing with a steel jacket, which was then coated with a thin dimensional galvanized chrome layer. This allowed Mazda to return to the 3mm and later even 2mm thick metal apex seals.Yamamoto, Kenichi (1971). Rotary Engine. Toyo Kogyo. Page 60-61 Another early problem was the build-up of cracks in the stator surface near the plug hole, which was eliminated by installing the spark plugs in a separate metal insert/ copper sleeve in the housing instead of a plug being screwed directly into the block housing.